effect of heating rate on the partial transient liquid
Post on 29-Jan-2017
Embed Size (px)
Association of Metallurgical Engineers of Serbia AMES
Scientific paper UDC: 669.711.058.6 ; 621.792.3:669.711
EFFECT OF HEATING RATE ON THE PARTIAL TRANSIENT LIQUID PHASE DIFFUSION BONDED Al/Mg2Si METAL MATRIX
COMPOSITE AND MAGNESIUM ALLOY (AZ91D) COUPLE
M. Mazar Atabaki , A.H. Meisami
1Institute for Materials Research, the School of Process, Environmental and Materials Engineering, Faculty of Engineering, University of Leeds, Leeds, UK
2Department of Materials Engineering, Faculty of Mechanical Engineering, Universiti Teknologi Malaysia, 81310, Malaysia
3Metallurgy & Material Dept., Golpayegan University of Technology, P.B.: 87717-65651, Golpayegan, Iran.
Received 26.09.2011 Accepted 07.11.2011
Abstract Partial transient liquid phase diffusion bonding of aluminium metal matrix
composite (Al/Mg2Si) and magnesium alloy (AZ91D) was performed using two heating rates. With an increase in heating rate from 2 to 20C/min, Mg content in the activated bond surface decreased and the microstructure was changed. The composition and microstructure of the joined areas were examined by X-ray diffraction (XRD) and scanning electron microscope (SEM) equipped with energy dispersive X-ray spectroscopy (EDS). Kinetics of the bonding process was accelerated due to the increase of solute diffusivity through grain boundaries of the metal matrix composite. Results suggest that Mg and Si contained in the interlayer favours the partial disruption of oxide films, giving superior creep resistance at high temperature.
Keywords: Metal-matrix composite; Magnesium alloy; Transient liquid phase
Introduction In the last decade, the need for lightweight materials has led to extensive efforts
in the improvement of aluminium metal matrix composites and magnesium alloys. Metal matrix composites were developed by the addition of various types of reinforcement particles to aluminium alloys with the intention of extending their applicability in electronic, aerospace, shipbuilding and automotive industries [1,2]. Corresponding author Mehdi Mazar Atabaki, firstname.lastname@example.org.
104 Metall. Mater. Eng. Vol 18 (2) 2012 p. 103-115
However, a new type of aluminium metal matrix composite (Al/Mg2Si) showed a potential as a replacement of lightweight alloys in automobile industries [3-5]. On the other hand, the use of magnesium alloys in the automotive applications continues to grow at an unprecedented rate. Among the magnesium alloys, AZ91D is increasingly being selected to replace aluminium, zinc and plastics as manufacturers strive to reduce component weight and production costs. These materials put high demands on the joining process because of their physical properties in the commercial applications. Development of a joining process for bonding of these materials is an essential step for their widespread industrial utilization. The conventional joining techniques are limited for bonding the aluminium metal matrix composite and the magnesium alloy for many reasons. For example, the magnesium alloy shows a relatively broad melting interval and this severely increases the risk of hot-cracking during the fusion welding. Another drawback with the fusion welding of the composite and the magnesium alloy is high viscosity and poor flowability of the liquid in the welding pool. This problem leads to a great mixing of the substrates with filler metal and accelerates the formation of deleterious phases in the bond region. In the conventional fusion welding methods, rejection of the reinforcement particles in the metal matrix composite during the solidification causes microsegregation and inhomogeneous distribution of the particles in the welding pool. As a consequence, there exist many defects and porosities in the fusion zone. In addition, using solid state joining techniques like friction stir welding often ended up with segregation and fragmentation of the reinforcement particles [6-10]. Recently, partial transient liquid phase diffusion bonding technique was applied for bonding some materials in critical applications [11-14]. In this process the design of a suitable interlayer for the system is the most important parameter.
This study concentrates on an approach to join Al/Mg2Si metal matrix composite to AZ91D by partial transient liquid phase diffusion bonding using a developed Al-base interlayer with 70m thickness. The study coupled with creep evaluation of the bonds at high temperature.
Experimental procedure In situ Al/Mg2Si composite was prepared using gravity casting technique by
melting commercial pure Al, Mg, Si and 15wt.% Mg2Si reinforcement particles with average diameter of 20 m. Casting was performed in an electric resistance furnace and the pouring temperature was 750C. Degassing was conducted for 6 minutes using dry tablets containing C2Cl6. After stirring, the molten composite was poured into a cast iron mould. The solidified composite was cut into 505025mm pieces by a wire cut machine. For preparing the magnesium alloy (AZ91D), commercial pure Mg, Al, Si, Zn and Mn were melted at 590C in an electric resistance furnace and then poured into a preheated steel mould to form ingots. Subsequently, the ingots were machined into the specimens with size of 502020mm. The Al-base interlayer was produced by melting the components at 710C in alumina crucible placed in an air furnace. The molten interlayer was stirred about 10 min using a ceramic coated steel impeller. The speed of the stirrer was maintained at 400 rpm. Then the melt was poured into a cast iron mould. The Al-base interlayer was rolled to reach the thickness of 70m. The nominal compositions of the materials are shown in Table 1.
Atabaki et al. Effect of heating rate on the partial transient liquid phase diffusion bonded... 105
Table 1. Chemical compositions of materials (wt.%).
Element Composition (wt. %) Material
Al Mg Si Fe Cu Zn Mn Cr Ni Ti V Al-Mg2Si-
Bal. 9.61 5.58 0.19 0.03 0.03 0.05 0.02 0.01 0.01 ---
9.3 Bal. 0.1 --- 0.025 0.45 0.15 --- 0.002 --- ---
Al-base interlayer Bal. 2.40 1.75 0.70 0.35 0.25 --- 0.35 --- 0.55 0.01
The composition of the interlayer was chosen to prevent the formation of
complicated intermetallic compounds, provide adequate mutual solubility and minimize the thermal expansion mismatch at the bond interface. The magnesium alloy comprises -Mg grains and Mg17Al12 at inter-dendritic boundaries while the composite contains binary eutectic -Al /Mg2Si, primary Mg2Si particles and -Al solid solution around the primary Mg2Si particles. Before the bonding process, the mating surface of the metal matrix composite and the magnesium alloy (10105 mm) were polished using 1200 grade emery paper, and ultrasonically cleaned in acetone.
The Al-base interlayer was inserted between two substrates and the specimens were assembled in a stainless steel fixture with a pressure of 0.5MPa. The bonding was carried out in a vacuum furnace maintained at 510-4 Pa. The bonding temperature was 400C. Before reaching to the bonding temperature the specimens were preheated at 300C. The key issue in this investigation was the use of different heating rates after preheating. Two heating rates (m1=2C/min and m2=20C/min) were set to break down the tenacious oxide layers at the faying surface of the specimens.
After the soaking time of 18 min at the bonding temperature, the specimens were cooled to service temperature (see Fig.1). The composition and microstructure of the bond regions were examined by scanning electron microscope (SEM) equipped with energy dispersive X-ray spectroscopy (EDS). Conventional compressive creep test was accomplished for the specimens with size 446 mm3. The test was performed at 350C under vacuum with applying a constant stress of 4 MPa.
106 Metall. Mater. Eng. Vol 18 (2) 2012 p. 103-115
Fig.1. Cycle of partial transient liquid phase diffusion bonding of Al-Mg2Si metal matrix
composite to AZ91D with Al-base interlayer. In the right side, concentration profile at the beginning of the solidification stage shows a temperature gradient (Gb) across the interface.
Results and discussion At the first stage of the process, the bonding temperature was selected under the
solidus line of the Al-base interlayer. After this stage, the bonding temperature was increased to the liquidus temperature of the interlayer. Holding the substrates at the third stage (tIII) causes the formation of different phases due to the diffusion routes in the bond region. Fig.2 shows the microstructure of the substrates bonded at two heating rates. It can be seen that although slight changes occurred at the faying surface of the substrates, the bonding process does not significantly alters the microstructure of the parent alloys.
Atabaki et al. Effect of heating rate on the partial transient liquid phase diffusion bonded... 107
Fig.2. SEM images of joints produced at heating rates of (a) 20 and (b) 2C/min for
bonding time of 18 min. The bonding temperature was 400C for both cases.
As it is seen, after interaction of the Al-based interlayer with the base materials, a
mutual diffusion of the alloying elements occurred. This lowered the melting temperature of the contact area compared to the bulk of the interlayer. It can be observed that a small amount of dissolution has happened between the interlayer and AZ91D substrate. The interface of the composite and the Al-base interlayer was planar while a thin sinusoidal diffusion layer was observed at the faying surface of AZ91D. The joints appeared to be sound, with low porosities in both interface areas. With ap